The fatigue behavior of cotton warps was studied by a newly weaving load simulator (WLS) developed in our laboratory. Reborn hairiness, strength retention, and elongation retention of sized warps were adopted to evaluate the physical and mechanical properties of sized warps under stretch-abrasion cyclic loading. The influences of different fatigue cycles on the above three indicators were also discussed. The results indicated that the fatigue behavior of the cotton warps accompanied by abrasion yields a three-parameter Weibull distribution. All the fitting plots show acceptable linearity. Moreover, there is a strong relationship of quadratic polynomial between the tensile properties and the fatigue cycle of the sized warps according to the scatter fitting (R^{2} > 91.08%). Similarly, there is also a good relationship of quadratic polynomial between the reborn hairiness index and the fatigue cycle of the sized warps (R^{2} > 94.51%). Finally, regardless of the strength retention, elongation retention, and reborn hairiness, the physical and mechanical properties of the cotton warps still change with the continuous increase of the fatigue cycle after 40% of the fatigue cycle, but it is not significant. The research was helpful to estimate the capacity of the warps to sustain failure.

#### Keywords

- Fatigue cycle
- three-parameter Weibull distribution
- physical and mechanical properties

The service performance of sized warps is mainly the fatigue characteristic of yarns, obviously affecting the appearance and properties of the fabric and consequently influencing the production efficiency. The property of sized yarns has proved a certain correlation with warp stop. The fatigue resistance of sized warps primarily depends on the properties of fiber component, spinning technology, sizing agent, chemical treatment technology, and weaving environment [1,2,3]. The tensile failure mechanism, under cyclic stretching, bucking, and axial abrasion, of yarns has been extensively studied by many researchers. Das worked on the tensile and abrasion behavior of blended spun yarn made on different spinning technologies [4]. However, Behera et al. studied the mechanical properties (such as cohesion power, adhesion power, abrasion resistance, and bending rigidity) of size films along with the weaving performance of the sized yarn [5]. Mokhtari et al. and Behera et al. reported on the fatigue fracture mechanism of yarn using a technique of digital image analysis [6, 7]. Seung et al. and Mishra et al. investigated the mechanical properties and abrasion behavior of yarn in fabric form [8, 9]. However, representing the fatigue characteristics of yarn based on the failure criterion in terms of only the fatigue cycle is not enough. The rate of fatigue damage expressed in terms of loss in tensile property indicators has also proven to be useful in assessing the fatigue-sustaining capacity of yarn and thereby predicting impending failure. Furthermore, the relevant literature on the characterization of physical and mechanical properties of sized warps under tensile fatigue loading is scarce, considering various factors.

The relationship between the fatigue cycles, loss in tensile properties, and gain in the physical properties of sized yarns must be balanced. Therefore, in this research, the effects of the fatigue cycle on strength retention (SR), elongation retention (ER), and reborn hairiness (RH) of sized warps by the WLS developed in our laboratory have been studied. To study the effect of the fatigue action on the tensile properties and physical characteristics of the sized warps, a detailed analysis was also performed. Besides, the failure characteristic of cotton warps was studied based on a three-parameter Weibull distribution. These findings not only presented the actual fatigue state and process of warps worn by a WLS but also better clarified the changes in the physical and mechanical properties of sized warps under a cyclic mechanic load. It was helpful to develop sized warps with higher weaving performance and estimate the capacity of the warps to sustain failure. Besides, the design of WLS comprehensively takes into account the fatigue characteristics of the yarn under a cyclic load of stretch abrasion.

The specimens used in this study were cotton compact spun yarns in common use, and a total of four specimens were selected to compare with the physical and mechanical properties. The specifications of the specimens are shown in Table 1.

Yarn specification

19.4 | 723.8 | 3.09 | 302.73 | 12.19 | 3.77 | 12.31 | 401.62 | 7.96 | 2.87 | 16.50 |

14.5 | 736.6 | 3.05 | 257.38 | 7.72 | 4.52 | 17.64 | 369.63 | 7.56 | 3.31 | 10.78 |

11.6 | 953.2 | 4.57 | 193.45 | 7.25 | 3.85 | 11.79 | 318.72 | 8.36 | 3.41 | 14.49 |

9.7 | 1002.3 | 2.78 | 187.74 | 6.19 | 3.95 | 34.26 | 262.73 | 10.05 | 3.15 | 14.23 |

The fatigue cycle tests of warps were conducted using the WLS developed in our laboratory. Figure 1 presents the schematic diagram of the simulator. One end of the warp was fixed to the pre-tension weight, and the other end passed through the splitting roller, and then through the drop and induction device, smooth roll, reciprocating friction roll, and the oscillating friction roll. The reciprocating friction roll imparted flex abrasion and cyclic stresses to yarn. The oscillating friction roll imparted only flex abrasion to yarn. During the test, the reciprocating friction roll and the oscillating friction roll reciprocated once, and they produced a tensile, friction, and buckling effect on the yarn. The internal counter of the simulator recorded the fatigue cycle once. The number of cycles required to break yarn in trials was the index of the fatigue cycle. Besides the deflection, characteristics of the friction roll such as its surface roughness and material size and shape may also affect fatigue resistance.

The testing parameters of the WLS including the load amplitude, load speed, and pre-tension were set to 70 mm, 180 cycle/min, and 2.1cN/tex, respectively. The temperature and the relative humidity were (20 ± 3)°C and (65 ± 5)%, respectively.

To investigate the effect of the fatigue test on the tensile properties, the sized warps were worn for a certain number of cycles on the WLS equal to 5, 10, 20, 40, and 80% of their fatigue cycles tested based on failure. The warps that survived after the above-mentioned fatigue levels were collected and the tensile properties were further measured using an electronic single yarn strength tester model SHIMADZU AGS-X according to GB/T 3916-1997 with 250 mm/min speed and 250 mm specimen length. Thirty tests were conducted for each sample and the mean values were acquired. The temperature and the relative humidity were (20 ± 3)°C and (65 ± 5)%, respectively. Equations (1) and (2) show the calculation of SR and ER, respectively. They are defined as follows:
_{1} is the breaking strength of worn warp in cN, and _{0} is the breaking strength of unworn warp in cN; ER is the elongation retention in %, _{1} is the elongation at break of worn warp in millimeter, and _{0} is the elongation at break of unworn warp in millimeter.

The RH of warps causes the warp ends to cling together and even break off when weaving. Particularly critical is RH in staple fibers when they are woven on air-jet looms. Therefore, RH is an important parameter to evaluate the physical property of warps after fatigue load. The WLS was developed for abrading yarn. In this article, specimens endured different fatigue cycles to examine the development of RH. The abrasion areas of the worn warps are marked and obtained. We used a yarn examine machine model YG381 manufactured by Nantong Hongda Experimental Instrument Co. LTD (Nantong, China) to wind the worn warps evenly on it. The scanner model 9000F Mark2 manufactured by Canon China Co. LTD (Shanghai, China) provided a digital image of yarn. Finally, the images were processed, and the hairiness area index was extracted from them by the developed program through MATLAB R2014b [10]. A total of 30 tests were conducted for each sample. The mean values and the coefficient of variation (CV) acquired were used as data. The hair area index (_{1}) was recorded. Hair area index (_{1}) is a unit-less parameter defined as a ratio between the total area of single (i.e. looped and protruding) fibers _{F} or _{F1} and the total area of core _{C} [11]. It can be expressed by the following equation:
_{F} is the total area of single fibers, _{C} is the total area of the core; _{1} is the hair (3 mm or longer) area index in %, and _{F1} is the area of single fibers (3 mm or longer).

The influence of linear density on the statistical distribution of the yarns’ fatigue characteristic was investigated by the Weibull distribution. The collected data on SR, ER, and RH were analyzed statistically by a scatter plot. Regression fitting and ^{2} were used to determine whether a response was significantly influenced by the independent parameters.

The behavior of Yarn fatigue follows a three-parameter Weibull distribution [12], which is given in Equation (5) as follows:

By taking the logarithm twice, Equation (5) can be rewritten in a linear form.

To evaluate the Weibull distribution model, a one-sample Kolmogorov–Smirnov (K–S) test was applied at a commonly adopted significance level (α = 0.01). The procedure of the goodness-of-fit test is as follows:

Determine the maximum deviation (_{n}) between _{0} from _{0} = (

The critical value _{nc} can be obtained from the K–S test table. For

If _{n} < _{nc}, the Weibull distribution model is considered as a significant fit to the observed distribution.

The fitting of the Weibull distribution model is effective, and the mean value and variance of Weibull distribution can be calculated as follows:

The fatigue characteristics of the yarn accompanied by strength and abrasion are of great importance for the weavability of warp. The Weibull distribution parameters of unsized and sized yarn samples in this article are given in Tables 2 and 3, respectively.

Weibull parameters of unsized yarn

19.4tex-S1 | 128 | 3.05 | 871.53 | 0.102 | 792.4 | 229.23 | 28.92% | |

14.5tex-S2 | 40 | 2.70 | 839.91 | 0.090 | 751.4 | 250.85 | 33.38% | |

11.6tex-S3 | 134 | 3.85 | 605.22 | 0.218 | 560.2 | 138.42 | 24.71% | |

9.7tex-S4 | 92 | 3.26 | 508.45 | 0.102 | 465.3 | 126.86 | 27.26% |

Weibull parameters of sized yarn

19.4tex-S5 | 162 | 2.81 | 1153.55 | 0.106 | 1045.1 | 309.36 | 29.60% | |

14.5tex-S6 | 210 | 2.53 | 1063.43 | 0.140 | 967.5 | 269.60 | 27.86% | |

11.6tex-S7 | 145 | 3.10 | 813.05 | 0.172 | 742.5 | 205.36 | 27.65% | |

9.7tex-S8 | 123 | 3.33 | 781.46 | 0.070 | 714.0 | 199.72 | 27.97% |

As for Figures 2(a) and 3(a), the Weibull statistical analysis of the fatigue cycle data yields three characteristic parameters for each group, that is, ^{2} > 0.919, except 11.6tex), signifying a reasonable Weibull distribution fitting. Furthermore, according to the values of _{n} using a one-sample K–S test, the fatigue cycle of the yarn at four different linear densities irrespective of unsized and sized yarns all fit the Weibull distribution well at a level of 1%: all the _{n} values are lower than that of the critical value (0.2305). As is well known, the twist imparted to the yarn affects the structure of yarn and the mechanical properties of the yarn. In automatic weaving, warp twist would also affect end breakage rate and consequently weaving efficiency. In general, increasing the twist and thus reducing the amount of loosely bound fiber on the yarn surface materially reduced the number of failures due to this factor. This is obviously due to the consolidation of the fiber assembly on account of the increase in helix angle, which causes an improvement in resistance to inter-fiber slippage during weaving stress. The twist level and linear density effects on the fatigue cycle of yarns are apparent, and the corresponding fatigue can be reasonably predicted from the three-parameter Weibull distribution model. The cumulative failure probability model (Figures 2(b) and 3(b)) is presented to predict the threshold values of the yarn fatigue cycle with different linear densities. All plots reveal a similar upward trend with increasing fatigue level, and yarns with different linear densities have different threshold values, which is a distinct indicator of the linear density dependence of the fatigue cycle. Therefore, the effect of linear density on the fatigue cycle cannot be ignored.

It can be also seen from Figure 2 that Weibull plots lie toward the far right of the plots for the yarn of 19.4 tex, followed by 14.5, 11.6, and 9.7 tex from right to left. This indicates the optimal fatigue property of the yarns of 19.4 tex as compared to that of the other three yarns, owing to the highest resistance to fatigue accompanied by stretch and abrasion. The higher the linear density of the yarn, the greater the number of fibers in the cross-section of yarn, and the harder it is to make it a failure. Nevertheless, after sizing, the improvement obtained in the weaving potential of yarn is substantially higher irrespective of linear density. These yarns exhibit similar trends after sizing, which are shown in Figure 3. Thus, it can be concluded that the fatigue characteristic of the yarn plays a dominant role in determining the weaving performance even in sized yarns.

Although the fatigue characteristic of yarn is of great importance for the warps, it is hard enough to establish weaving potential in terms of the characteristic fatigue cycle calculated by fitting a Weibull distribution because the actual tensile fatigue cycles of the yarn imposed on a loom can sometimes be far lower than these characteristic fatigue cycles. Therefore, understanding the gradual deterioration of yarn tensile properties as fatigue levels increase may yield useful information about the potential failure of yarn. Moreover, the breaking strength and breaking elongation of a warp are reduced by about 10% after weaving [14]. SR of a warp was a parameter that can reflect the ability to avoid damage from failure [15, 16]. In this experiment, with four sized yarn of different linear densities, the relationship between the SR and fatigue cycles as well as between ER and fatigue cycles was studied.

The variations in SR and ER with four sized warps of different linear densities are shown in Figure 4. As can be shown, both the SR and ER decrease generally with increasing fatigue cycles, as expected. Figure 4(a) shows that the SRs drop slightly in the first 5% of fatigue cycles, especially for 14.5tex yarn from 100% to 96.73%. This may be explained as follows. At the initial testing stage, a small amount of the size coating gets abraded, residual surface slurry maintained the structural integrity of warp and played a role in protecting fibers. Therefore, the reduction of yarn strength is not obvious. With the test progressing, the surface slurry was gradually worn off, and the exposed sheath fibers were worn directly by the load component. Cracks occurred on the surface of fibers and they damaged the structural integrity of the warps, which resulted in a decrease in the tensile properties [17]. Thus, the SR of yarns steadily declines from 100% to below 90.09% in the first 10% of fatigue cycles, except 14.5 tex yarn. Figure 4(a) also demonstrated that SR declined significantly from 20% to 40% of the fatigue cycle. The reason is that the warp was always kept in close contact with the load component and damaged after being worn for a certain amount of cycles. Once the relative movement between the warp and the load component occurred, the repetitive load between sheath fibers of warp and the load component would greatly reduce the cross-section and lead to a sharp decrease in tensile properties of warp [18, 19]. Moreover, in each fatigue cycle of the test, the testing area of warp alternated between straight and curved conditions, which caused bending and tensile fatigue. The indicator of ER shows a similar tendency, as shown in Figure 4(b). The results also reveal that the SR and ER of the yarn do not continuously decrease with increasing fatigue cycles but reach a threshold value at a 40% of fatigue cycle, after which they start to decline slowly. The authors observed a similar trend for cotton yarns [2, 6, 20]. Figure 4 also demonstrates a very strong relationship of quadratic polynomials between the tensile property and the fatigue cycle. The results of ^{2} are all within the acceptable range. Therefore, in practical applications, the critical issue is to improve the surface performance of warp to reduce the influence of abrasion and stretch on its mechanical properties.

The RH of yarn is an important index to evaluate the physical performance of yarn. Reducing the RH generated during weaving can effectively avoid end-breakage caused by the adhesion between adjacent warps. The relationships between fatigue cycle and hair area index as well as between the fatigue cycle and hair area index (3mm or longer) are shown in Figure 5. According to the experimental results and observed morphology, typical images of worn warps at various fatigue cycles were obtained, as shown in Table 4.

Initial images and images after each fatigue cycle

As can be seen in Figure 5, under different fatigue cycles, _{1} indicate that the RH increases slightly with an increasing fatigue cycle in the first 5% of fatigue cycles for all samples mentioned above. This may be explained as follows. First, a thin layer of the size coating is abraded, the friction component had worn off the surface of sheath fibers and exposing surface fibers of yarns to abrasion to generate a small amount of hairiness. Similarly, RH has been found to increase gradually with the increase of the fatigue cycle from 5% to 20%. The presence of worn warp gradually progressed from slightly fuzzy to rough in this stage. Nevertheless, plucking of fibers from the yarn body due to cycle abrasion and stretch is likely to create higher RH in the sheath between 20% and 40% of the fatigue cycle. Therefore, the RH is almost twice the amount suffered by up to 40% of the fatigue cycle. It is especially obvious for the ^{2} are almost all above 95.50%. The uptrend of RH increasing with the fatigue cycle coincides with the downtrend of SR decreasing with fatigue life.

This article studied the physical and mechanical properties and fatigue characteristics of cotton warps. According to the experimental results and analysis, the following conclusions can be drawn.

The fatigue behavior of cotton warps accompanied by abrasion yields a three-parameter Weibull distribution. All the fitting plots show acceptable linearity.

Fatigue action can significantly reduce the tensile properties and enhance the RH of sized warps. According to the scatter fitting, there are both strong relationships of quadratic polynomial between the tensile properties and the fatigue cycle of the sized warps as well as between the RH index and the fatigue cycle of the sized warps. The results of ^{2} of all fitting models are almost above 95.50%.

The physical and mechanical properties of the cotton warps still change with the continuous increase of the fatigue cycle beyond 40% of the fatigue cycle. Nevertheless, the changing trend is not significant.

#### Yarn specification

19.4 | 723.8 | 3.09 | 302.73 | 12.19 | 3.77 | 12.31 | 401.62 | 7.96 | 2.87 | 16.50 |

14.5 | 736.6 | 3.05 | 257.38 | 7.72 | 4.52 | 17.64 | 369.63 | 7.56 | 3.31 | 10.78 |

11.6 | 953.2 | 4.57 | 193.45 | 7.25 | 3.85 | 11.79 | 318.72 | 8.36 | 3.41 | 14.49 |

9.7 | 1002.3 | 2.78 | 187.74 | 6.19 | 3.95 | 34.26 | 262.73 | 10.05 | 3.15 | 14.23 |

#### Weibull parameters of sized yarn

19.4tex-S5 | 162 | 2.81 | 1153.55 | 0.106 | 1045.1 | 309.36 | 29.60% | |

14.5tex-S6 | 210 | 2.53 | 1063.43 | 0.140 | 967.5 | 269.60 | 27.86% | |

11.6tex-S7 | 145 | 3.10 | 813.05 | 0.172 | 742.5 | 205.36 | 27.65% | |

9.7tex-S8 | 123 | 3.33 | 781.46 | 0.070 | 714.0 | 199.72 | 27.97% |

#### Weibull parameters of unsized yarn

19.4tex-S1 | 128 | 3.05 | 871.53 | 0.102 | 792.4 | 229.23 | 28.92% | |

14.5tex-S2 | 40 | 2.70 | 839.91 | 0.090 | 751.4 | 250.85 | 33.38% | |

11.6tex-S3 | 134 | 3.85 | 605.22 | 0.218 | 560.2 | 138.42 | 24.71% | |

9.7tex-S4 | 92 | 3.26 | 508.45 | 0.102 | 465.3 | 126.86 | 27.26% |

Apparel Industry in the EU–China Exports and Circular Economy Automatic Identification Of Wrist Position In A Virtual Environment For Garment Design Pressure Evaluation Of Seamless Yoga Leggings Designed With Partition Structure Experimental and Modelling Studies on Thermal Insulation and Sound Absorption Properties of Cross-Laid Nonwoven Fabrics Tensile Properties Analysis Of 3D Flat-Knitted Inlay Fabric Reinforced Composites Using Acoustic Emission Optimization of Sodium Lignosulfonate Treatment on Nylon Fabric Using Box–Behnken Response Surface Design for UV Protection A Study on the Woven Construction of Fabric Dyed With Natural Indigo Dye and Finishing for Applying to Product Design for Home Textile Products A Calculation Method for the Deformation Behavior of Warp-Knitted Fabric Nondestructive Test Technology Research for Yarn Linear Density Unevenness Numerical Simulation and Analysis of Airflow in the Condensing Zone of Compact Spinning with Lattice Apron Blend Electrospinning of Poly(Ɛ-Caprolactone) and Poly(Ethylene Glycol-400) Nanofibers Loaded with Ibuprofen as a Potential Drug Delivery System for Wound Dressings Application of Plasticized Cellulose Triacetate Membranes for Recovery and Separation of Cerium(III) and Lanthanum(III) Analysing Service Quality and its Relation to Customer Satisfaction and Loyalty in Sportswear Retail Market A Review on the Performance and Comfort of Stab Protection Armor A Fabric-Based Integrated Sensor Glove System Recognizing Hand Gesture Developing Real Avatars for the Apparel Industry and Analysing Fabric Draping in the Virtual Domain Simulations of Heat Transfer through Multilayer Protective Clothing Exposed to Flame Determination of Sewing Thread Consumption for 602, 605, and 607 Cover Stitches Using Geometrical and Multi-Linear Regression Models Evaluation of Functional Insoles for Protective Footwear Under Simulated Use Conditions Designing a Three-Dimensional Woven Fabric Structure as an Element of a Baby Stroller Computer-Assisted Modeling and Design of Compression Garments with Graded Unit Compression Application of Physical Vapor Deposition in Textile Industry Modeling Lean and Six Sigma Integration using Deep Learning: Applied to a Clothing Company Comparative Analysis of Structure and Properties of Stereoscopic Cocoon and Flat Cocoon Effect of Water pH on Domestic Machine Washing Performance of Delicate Textiles Effect of Different Yarn Combinations on Auxetic Properties of Plied Yarns Analysis of Heat Transfer through a Protective Clothing Package Smart Textile for Building and Living Investigation of Twist Waves Distribution along Structurally Nonuniform Yarn 3D Body Scan as Anthropometric Tool for Individualized Prosthetic Socks Preliminary Experimental Investigation of Cut-Resistant Materials: A Biomimetic Perspective Durable Wash-Resistant Antimicrobial Treatment of Knitted Fabrics Modeling Supply Chain Sustainability-Related Risks and Vulnerability: Insights from the Textile Sector of Pakistan Numerical Simulation of Fiber Motion in the Condensing Zone of Lateral Compact Spinning with Pneumatic Groove Study on the Thermal and Impact Resistance Properties of Micro PA66/PU Synergistically Reinforced Multi-Layered Biaxial Weft Knitted Fabric Composites Improvement of Physical Properties of Viscose Using Nano GeO _{2}as Doping MaterialFea-Based Structural Heat Transfer Characteristic of 3-D Orthogonal Woven Composite Subjected to the Non-Uniform Heat Load Bending Failure Behavior of the Glass Fiber Reinforced Composite I-Beams Formed by a Novel Bending Pultrusion Processing Technique Comfort-Related Properies of Cotton Seersucker Fabrics Economical and Social Dimensions of Unionization in Turkish Textile and Clothing Sector Conductive Heat Transfer Prediction of Plain Socks in Wet State A Novel Foam Coating Approach to Produce Abrasive Structures on Textiles Textronic Solutions Used for Premature Babies: A Review Effect of Lycra Weight Percent and Loop Length on Thermo-physiological Properties of Elastic Single Jersey Knitted Fabric Texture Representation and Application of Colored Spun Fabric Using Uniform Three-Structure Descriptor Analysis of Mechanical Behavior of Different Needle Tip Shapes During Puncture of Carbon Fiber Fabric Approach to Performance Rating of Retroreflective Textile Material Considering Production Technology and Reflector Size Influence of Multilayer Interlocked Fabrics Structure on their Thermal Performance Prediction of Standard Time of the Sewing Process using a Support Vector Machine with Particle Swarm Optimization A Novel Theoretical Modeling for Predicting the Sound Absorption of Woven Fabrics Using Modification of Sound Wave Equation and Genetic Algorithm Ag Coated Pa-Based Electro-Conductive Knitted Fabrics for Heat Generation in Compression Supports Design Method of Circular Weft-Knitted Jacquard Fabric Based on Jacquard Module Image Analysis as a Method of the Assessment of Yarn for Making Flat Textile Fabrics Investigation of Heat Transfer in Seersucker Woven Fabrics using Thermographic Method Research into the Textile-Based Signal Lines Made Using Ultrasonic Welding Technology Transformable Warning Clothing for Children with Active Light Sources Regenerated Cellulose/Graphene Composite Fibers with Electroconductive Properties High-Performance Workwear for Coal Miners in Northern China: Design and Performance Evaluation Comfort-Related Properties of Double-Layered Woven Car Seat Fabrics Experimental Investigation of the Wettability of Protective Glove Materials: A Biomimetic Perspective An Integrated Lean Six Sigma Approach to Modeling and Simulation: A Case Study from Clothing SME Mechanical Properties of Composites Reinforced with Technical Embroidery Made of Flax Fibers Consumer Adoption of Fast-Fashion, Differences of Perceptions, and the Role of Motivations Across the Adoption Groups A New Consumer Profile Definition Method Based on Fuzzy Technology and Fuzzy AHP Optimal Design of a Novel Magnetic Twisting Device Based on NSGA-II Algorithm Microscopic Analysis of Activated Sludge in Industrial Textile Wastewater Treatment Plant Evaluation of Physical and Mechanical Properties of Cotton Warps Under a Cyclic Load of Stretch-Abrasion Theoretical and Experimental Evaluation of Thermal Resistance for Compression Bandages Effects of Flocks Doping on the Dynamic Mechanical Properties of Shear Thickening Gel Estimation of Seams in Paraglider Wing Sensitivity of Aerodynamic Characteristics of Paraglider Wing to Properties of Covering Material Numerical Investigation of Heat Transfer in Garment Air Gap Determination of State Variables in Textile Composite with Membrane During Complex Heat and Moisture Transport Design and Performance Evaluation of Protective Clothing for Emergency Rescue Biological Properties of Knitted Fabrics Used in Post-Burn Scar Rehabilitation Fabrication and Characterization of Fibrous Polycaprolactone Blended with Natural Green Tea Extracts Using Dual Solvent Systems